4 Ultimate AnalysisThe ultimate analysis of coal involves determination of the weight percentcarbon as well as sulfur, nitrogen, and oxygen (usually estimated by difference).Trace elements that occur in coal are often included as a part of the ultimateanalysis.The carbon determination includes carbon present as organic carbon occurringin the coal substance and any carbon present as mineral carbonate. The hydro-gen determination includes hydrogen present in the organic materials as well ashydrogen in all of the water associated with the coal (Chapter 3). In the absenceof evidence to the contrary, all of the nitrogen is assumed to occur within theorganic matrix of coal. On the other hand, sulfur occurs in three forms in coal:(1) as organic sulfur compounds; (2) as inorganic sulﬁdes that are, for the mostpart, primarily the iron sulﬁdes pyrite and marcasite (FeS2); and (3) as inorganicsulfates (e.g., Na2SO4, CaSO4). The sulfur value presented for ultimate analysismay include, depending on the coal and any prior methods of coal cleaning,inorganic sulfur and organic sulfur.Moisture and ash (Chapter 3) are not determined as a part of the data pre-sented for ultimate analysis but must be determined so that the analytical valuesobtained can be converted to comparable bases other than that of the analysissample. In other words, analytical values may need to be converted to an as-received basis, a dry basis, or a dry, ash-free basis. When suitable correctionsare made for any carbon, hydrogen, and sulfur derived from the inorganic mate-rial, and for conversion of ash to mineral matter, the ultimate analysis representsthe elemental composition of the organic material in coal in terms of carbon,hydrogen, nitrogen, sulfur, and oxygen.The standard method for the ultimate analysis of coal and coke (ASTM D-3176) includes the determination of elemental carbon, hydrogen, sulfur, andnitrogen, together with the ash in the material as a whole. Oxygen is usuallycalculated by difference. The test methods recommended for elemental analy-sis include the determination of carbon and hydrogen (ASTM D-3178), nitrogen(ASTM D-3179), and sulfur (ASTM D-3177; ISO 334; ISO 351), with associateddetermination of moisture (ASTM D-3173) and ash (ASTM D-3174) to convertthe data to a moisture-ash-free basis.Handbook of Coal Analysis, by James G. SpeightISBN 0-471-52273-2 Copyright 2005 John Wiley & Sons, Inc.67
68 ULTIMATE ANALYSIS4.1 CARBON AND HYDROGENCarbon and hydrogen, which, respectively, account for 70 to 95% and 2 to 6% byweight (dry, ash-free) of the organic substance of coal, are thought by some to bethe most important constituents of coal. Almost all of the carbon and hydrogenin coal occurs in combined form in the complex organic compounds that makeup coal. But carbon also occurs in the mineral carbonates, with calcite beingthe principal component, and hydrogen is also present in the various forms ofmoisture found in coal.4.1.1 Test Method ProtocolsAll methods of determining the carbon and hydrogen content of coal are verysimilar insofar as elemental carbon and hydrogen is determined by combustion ina closed system (combustion train), and the products of combustion are collectedin an absorption train. The percentages by weight of carbon and hydrogen arecalculated from the gain in weight of the relevant segments of the absorptiontrain. This method gives the total percentages of carbon and hydrogen in thecoal, including any carbon in the carbonates and any hydrogen in free moistureand in water of hydration of silicates. Reporting hydrogen and oxygen in thefree water (moisture) associated with the sample may optionally be included orexcluded from the hydrogen and oxygen values. The test method recommendsmaking a notation of the option (as received, or dry, or dry, ash-free) used asthe basis for reporting results. Hydrogen in the water of hydration of silicates isgenerally ignored but can introduce errors for coals that contain high amounts ofmineral matter. Overall, it is preferable, therefore, that the hydrogen and oxygenassociated with the free moisture not be included in the hydrogen and oxygenvalues and that moisture be reported as a separate item.Several automated elemental analysis systems suitable for coal analyses allowsimultaneous determination of carbon, hydrogen, and nitrogen for multiple sam-ples. In fact, rather than by difference (which also accumulates all the errorsof other determinations), oxygen can be determined using a separate combus-tion system. The systems convert coal (catalytically) to nitrogen, carbon dioxide,and water, which are separated with a gas chromatographic column and detectedthrough a sensor, such as a dual thermal conductivity cell. Sulfur can be deter-mined using a similar system that excludes the oxygen determination.In practice, the older well-used methods (ASTM D-3178; ISO 609; ISO 625)for determining carbon and hydrogen involve combustion of an exact amount ofthe coal in a closed system and the products of the combustion (carbon dioxideand water) determined by absorption. The combustion is usually accomplished byplacing the ground coal (to pass through, for example, a 60-mesh/250-µm sieve)in a stream of dry oxygen at temperatures on the order of 850 to 900◦C (1560to 1650◦F) (ASTM D-3178). Complete conversion of the combustion gases tocarbon dioxide and water can be achieved by passing the gases through heatedcupric oxide.
CARBON AND HYDROGEN 69As noted above, the equipment used for determination of the carbon andhydrogen content of coals consists basically of two parts: a combustion unit andan absorption train (ASTM D-3178). The combustion unit is made up of threeseparate electrically heated furnaces and the combustion tube. The ﬁrst furnace,at the inlet end of the tube, is approximately 130 mm long and can be movedalong the tube. The second and third furnaces are 330 mm and 230 mm in length,respectively, and are mounted in a ﬁxed position around the combustion tube.The required operating temperatures are 850 to 900◦C (1562 to 1652◦F), 850 ±20◦C (1562 ± 36◦F), and 500 ± 20◦C (932 ± 36◦F) for the ﬁrst, second, andthird furnaces, respectively. The combustion tube can be constructed from fusedquartz or high-silica glass. The combustion tube is packed with lead chromate(PbCrO3) or silver (Ag) gauze under the third furnace and cupric oxide (CuO)under the second furnace. Oxidized copper gauze plugs are used to contain thesecomponents in the tube.The absorption train is composed of a tube packed with water absorbent, asecond tube packed with a carbon dioxide absorbent, and a guard tube packedwith equal volumes of the water and carbon dioxide absorbents. Anhydrous mag-nesium perchlorate (MgClO4) is commonly used for the water absorbent, whilesodium hydroxide (NaOH) or potassium hydroxide (KOH) impregnated in aninert carrier is used as the carbon dioxide absorber.In the analytical procedure, a weighed amount of coal is placed in either a boat(glazed porcelain, fused silica, or platinum) and inserted into the combustion tubeunder the ﬁrst furnace, where the sample is burned in oxygen. The combustionproducts are allowed to ﬂow over the heated copper oxide and lead chromate orsilver and into the absorption train. The copper oxide ensures complete combus-tion of the carbon and hydrogen in the coal, whereas the lead chromate absorbsthe oxides of sulfur. If silver gauze is used, both the sulfur oxides and chlorinewill be absorbed. The preweighed absorbers in the absorption train absorb waterand carbon dioxide, and the percent of carbon and hydrogen in the sample iscalculated from the gain in weight of absorbers.This particular method of combustion analysis for carbon and hydrogen (Liebigmethod) is used internationally, although some modiﬁcations may have beenmade by the various national standards organizations. The sample size can varyfrom as little as 1 to 3 mg (microanalysis) to 100 to 500 mg (macroanalysis) withcombustion temperatures as high as 1300◦C (2370◦F). However, the method mustensure complete conversion of all of the carbon in the coal to carbon dioxideand all of the hydrogen to water. Oxides of sulfur and chlorine are removed bypassing the products of combustion over heated lead chromate and silver gauze.The carbon (as carbon dioxide) and hydrogen (as water) are calculated fromthe increase in weight of the absorbents used to collect the water and carbondioxide. Oxides of sulfur (and chlorine, which may be released in signiﬁcantamounts) are usually removed from the combustion gases by passage over silverat about 600◦C (1110◦F) while nitrogen dioxide is removed by lead chromateor manganese dioxide. The preliminary and ﬁnal procedure involves the passage
70 ULTIMATE ANALYSISof dry air (also free of carbon dioxide) through the system in order that theabsorption train may be weighed full of air before and after the determination.It is essential that both air and oxygen be pure. If not, puriﬁcation can beassured by passage through a puriﬁcation train consisting of (1) 30% aqueoussolution of potassium hydroxide, (2) concentrated sulfuric acid, and (3) two U-tubes charged with soda lime (or other dry absorbent for carbon dioxide) andcalcium chloride. It may be advisable to use two puriﬁcation trains (one for eachgas) leading to a common tube for delivery to the combustion train.Usually, the coal burns smoothly in the stream of oxygen. However, if thecombustion unit used for burning the sample is heated too rapidly, volatile mattermay be released at such a rate that some of it may pass through the entire systemand not be completely burned or absorbed. To prevent this from happening, thetemperature of the combustion unit must be at the proper level, and enough timemust be allowed for complete combustion. In addition, a proper ﬂow of oxygenmust be maintained through the system.The formation of oxides of nitrogen during the combustion process may leadto slightly high results for carbon and hydrogen, since the oxides are acidicin nature and would be absorbed in the absorption train. There are indicationsthat the hydrogen value would not be greatly inﬂuenced but that the carbonvalue would be higher by an amount depending on the nitrogen content andthe nitrogen oxides formed during the combustion. For more precise results, theoxides of nitrogen can be removed by absorption on manganese dioxide, or insome cases lead dioxide, before absorption of the water and carbon dioxide.However, caution is advised in treating any potential error lightly.Since inorganic carbonates and nitrogen oxides contribute to the carbon valuein coal as it is normally determined, consideration of this issue is necessary.Hydrogen values also are usually high, due to the inclusion of the various formsof moisture that are present in coal. All of these factors limit the reliability ofcarbon and hydrogen data for predicting the amount of combustible carbon andhydrogen in coal.Finally, and most important, blank determinations should be carried out atregular intervals.4.1.2 Data Handling and InterpretationIf the coal is not dried, the water collected in the adsorption train also containswater present originally as moisture in the coal (Chapter 3). The hydrogen equiv-alent to the percentage of moisture in the coal is deducted from the percentage ofhydrogen given by the method described above to arrive at the corrected ﬁgure,or alternatively, the quantity of moisture present in the weight of coal used is sub-tracted from the weight collected in the calcium chloride tube before calculatingthe equivalent weight of hydrogen burned.Subtracting one-ninth of the determined moisture from the determined hydro-gen can make a reasonable correction to the hydrogen value for the moisturein coal. A correction to the hydrogen value for the water of hydration of min-eral matter is more difﬁcult. The water of hydration of mineral matter for some
NITROGEN 71(U.S.) coals has been estimated to be 8% of the ash value. A correction of thehydrogen value for the water of hydration can thus be estimated by multiplyingthe ash value by 0.08, and one-ninth of this ﬁgure will give the correction to besubtracted from the hydrogen determined. Upon making these corrections for theforms of moisture, the value for the hydrogen can be calculated:H = Has-determined −2.0218.02 Mas-determined + 8100× Aas-determined(4.1)where H is hydrogen, M moisture, and A ash.The results of the carbon and hydrogen analysis may be reported on any num-ber of bases, differing from each other in the manner by which moisture valuesare treated. Inclusion of the hydrogen of moisture and water of hydration of min-eral matter in the hydrogen value is common practice for the as-determined andas-received bases. Hydrogen values on a dry coal basis, however, are commonlycorrected for the hydrogen of moisture. No corrections are normally made to thedetermined hydrogen value for the water of hydration of mineral matter, due tothe uncertainty of the estimate of its value.4.2 NITROGENNitrogen occurs almost exclusively in the organic matter of coal. Very littleinformation is available concerning the nitrogen-containing compounds present incoal, but they do appear to be stable and are thought to be primarily heterocyclic.The original source of nitrogen in coal may have been both plant and animalprotein. Plant alkaloids, chlorophyll, and other porphyrins contain nitrogen incyclic structures stable enough to have withstood changes during the coaliﬁcationprocess and thus to have contributed to the nitrogen content of coal.4.2.1 Test Method ProtocolsThe standard procedure of nitrogen determination by many laboratories isthe Kjeldahl method (ASTM D-3179; ISO 333), although there are thestandard methods that involve the Dumas technique (DIN 51722) and thegasiﬁcation procedure (DIN 15722). Neutron activation analysis has also beenproposed for the determination of nitrogen in coal, coal ash, and relatedproducts (Volborth, 1979a).In the Kjeldahl method, pulverized coal is boiled coal with concentrated sul-furic acid containing potassium sulfate and a suitable catalyst to reduce the timefor digestion. The catalyst is usually a mercury salt, selenium itself, or a seleniumcompound, or a mixture of the two. Selenium is regarded as being particularlyadvantageous.The Kjeldahl–Gunning macro method is the one most widely used for deter-mining nitrogen (ASTM D-3179). By this method, any nitrogen present in the
72 ULTIMATE ANALYSISsample is converted into ammonium salts by the destructive digestion of the sam-ple by a hot mixture of concentrated sulfuric acid and potassium sulfate. After thedigestion mixture has been made alkaline with sodium or potassium hydroxide,ammonia is expelled by distillation, condensed, and absorbed into a sulfuric acidsolution and the excess acid is titrated with sodium hydroxide solution. The alter-native method is similar except that after the complete digestion, the ammoniais distilled into a boric acid solution and titrated with a standard acid solution.Proper precautions should be taken in carrying out this procedure, especially thedigesting and distillation steps. In addition to the possibility of losing nitrogen-containing species if the proper heating rate is not observed, there is the problemof working with hot concentrated sulfuric acid and caustic solutions.A catalyst is used in the Kjeldahl–Gunning method to increase the rate ofdigestion of the coal and hence shorten the digestion period. For most bitumi-nous and low-rank coals, the digestion period is on the order of 3 to 6 hours, evenwith the aid of a catalyst, and anthracite may require as much as 12 to 16 hours.A variety of catalysts can be used, including mercuric sulfate (HgSO4) and sele-nium, mercuric selenite (HgSeO3), or cupric selenite dihydrate (CuSeO4 · 2H2O).However, when a mercury-containing catalyst is used, the addition of potassiumor sodium sulﬁde (Na2S) to the digestion mixture is necessary. The sulﬁde ionsprecipitate any mercuric ions as mercuric sulﬁde (HgS) and prevent formation ofa stable mercury–ammonia complex ion (ammonia is produced in the reaction).The most serious issue associated with the use of the Kjeldahl–Gunningmethod is whether or not complete conversion of nitrogen in the nitrogenouscompounds to ammonia occurs. The main reason is that complete conversionmay not be accomplished, for several reasons. The chemistry is more complexif not always straightforward, and in the presence of various oxidizing agents,nitrogen can be oxidized to nitrogen oxides which may be lost from the analy-sis. In addition, pyridine carboxylic acids may be formed, and these compoundsare resistant to further decomposition. Thus, the somewhat limited oxidationand digestion conditions and the possible formation of unwanted but stable by-products usually require a lengthy digestion period. In many cases, to ensurecomplete conversion of the nitrogen to ammonia, the addition of chromic oxide(Cr2O3) to the digestion mixture increases the rate of digestion of coke.The semimicro Kjeldahl–Gunning method (ASTM D-3179; ISO 333) hasbecome a widely used method for determining nitrogen in coal, but there is somedoubt about whether or not nitrogen recovery is complete by this procedure. Infact, the fate of nitrogen in the Kjeldahl method depends on its chemical formin the coal, the inorganic compounds added to catalyze the hydrolysis, and theamounts and types of compounds used to raise the boiling point of the mixture.The Dumas method of nitrogen determination consists of an oxidation methodin which a mixture of coal and copper oxide (CuO) is heated in an inert atmo-sphere to produce carbon dioxide (CO2), water (H2O), and nitrogen (N2). Thecarbon dioxide is absorbed, the water condensed, and the nitrogen determinedvolumetrically. Although the Dumas method has been employed for many years,various modiﬁcations have been made to increase accuracy and precision.
SULFUR 73The gasiﬁcation method consists of mixing coal with a mixture of two parts ofthe Eschka mixture (i.e., 67% w/w light calcined magnesium oxide and 33% w/wanhydrous sodium carbonate), six parts of soda lime, and one part of molybdenumoxide. The sample is then placed in a porcelain boat, covered with platinum gauze,and heated (in a quartz tube) to 200 to 250◦C (392 to 482◦F). The sample is thenheated in steam at 850 to 950◦C (1562 to 1742◦F). The gases pass into 0.1 Nsulfuric acid, where ammonia is chemically absorbed as ammonium sulfate andthen determined by one of the usual techniques.Nitrogen determination by perchloric acid digestion of coal without catalystsis reportedly safe and much more rapid than the conventional Kjeldahl procedure.Nitrogen is determined in the digest by the usual ammonia evolution and titration.However, extreme care should be taken whenever perchloric acid is used. Nuclearreactions have been applied successfully to the determination of nitrogen in coal.Nuclear reactions have been applied successfully to the determination of nitro-gen in coal. Coal has been irradiated with fast neutrons from a 14-MeV generatorto produce 13N, which decays via positron emission and has a 10-minute half-life.Standard deviation for the nitrogen determinations was 0.07%. The instrumen-tal neutron activation values were 6.8% higher (0.1% N) on average than thoseobtained using the standard Kjeldahl procedure. In the Kjeldahl procedure, lossof elemental nitrogen or nitrogen oxides or resistant heterocyclic nitrogen com-pounds can sometimes cause data errors, although most of these have beeneliminated by application of modern laboratory procedures. Because results frominstrumental neutron activation for nitrogen are independent of these factors, ithas been suggested that the activation method is the more accurate of the two.4.2.2 Data Handling and InterpretationNitrogen data are used primarily in research and for the comparison of coals.These values are needed so that the oxygen content of a coal can be estimated bydifference. During combustion, the nitrogen in coal can be converted to ammonia,elemental nitrogen, or nitrogen oxides, depending on the conditions of burningand the nature of the coal used. Nitrogen values could possibly be used to estimatethe amount of nitrogen oxides that would be emitted upon burning of certaincoals. Coal nitrogen values are also useful in predicting the amount of nitrogenin the products of coal liquefaction and gasiﬁcation processes.4.3 SULFURSulfur is an important consideration in coal utilization, and hence, there is aconsiderable amount of published work relating to the development of methodsto improve the efﬁciency of the techniques as well as improve the accuracy andprecision of the sulfur determination (Ahmed and Whalley, 1978; Chakrabarti,1978a; Attar, 1979; Raymond, 1982; Gorbaty et al., 1992).Total sulfur data (ASTM D-3177; ASTM D-4239) are necessary for the effec-tive control of the emissions of oxides of sulfur whenever coal is used as a fuel.
74 ULTIMATE ANALYSISThe emission of sulfur oxides leads to the corrosion of equipment and slagging ofcombustion or boiler equipment, as well as contributing to atmospheric pollutionand environmental damage. Sulfur data are therefore necessary for the evaluationof coals to be used for combustion purposes.Most coal conversion and cleaning processes require two sets of sulfur values:the sulfur content of the coal before it is used and the sulfur content of theproducts formed. In the coking of coal, some of the sulfur is removed in thecoking process, which makes it necessary to obtain the before and after values.The commercial uses of coke, as in metallurgical processes, require a low sulfurcontent and necessitate an accurate sulfur value for the coke. In coal gasiﬁcationand liquefaction processes, the sulfur in the coal is sometimes carried through tothe products. It is therefore necessary to determine the amount of sulfur in eachof the products before it is used. One of the primary reasons for cleaning coalis to reduce the sulfur content. It is necessary to know the sulfur content beforeand after cleaning in order to evaluate the cleaning process.Total sulfur values alone are not adequate in accessing a cleaning process forreducing the sulfur content of coal. Pyrite sulfur alone can be removed by speciﬁcgravity separations, and its removal depends on the way the pyrite is distributedthroughout the coal. If it occurs as very small crystals widely dispersed in the coal,it is almost impossible to remove by these methods. When pyrite occurs in largepieces, it can be removed successfully by speciﬁc gravity methods. Organic sulfurcannot be reduced appreciably, since it is usually uniformly dispersed throughoutthe organic material in coal.Sulfur is present in coal in three forms, either as (1) organically bound sulfur,(2) inorganic sulfur (pyrite or marcasite, FeS2), or (3) inorganic sulfates (ASTMD-2492; ISO 157; Kuhn, 1977). The amount of organic sulfur is usually <3%w/w of the coal, although exceptionally high amounts of sulfur (up to 11%) havebeen recorded. Sulfates (mainly calcium sulfate, CaSO4, and iron sulfate, FeSO4)rarely exceed 0.1% except in highly weathered or oxidized samples of coal. Pyriteand marcasite (the two common crystal forms of FeS2) are difﬁcult to distinguishfrom one another and are often (incorrectly) designated simply as pyrite. Freesulfur as such does not occur in coal to any signiﬁcant extent. The amount of thesulfur-containing materials in coal varies considerably, especially for coals fromdifferent seams. In addition, pyrite is not uniformly distributed in coal and canoccur as layers or slabs or may be disseminated throughout the organic material asvery ﬁne crystals. The content of sulfates, mainly gypsum (CaSO4 · 7H2O) andferrous sulfate (FeSO4 · 7H2O), rarely exceeds a few hundredths of a percent,except in highly weathered or oxidized coals.4.3.1 Test Method ProtocolsThe three most widely used test methods for sulfur determination are (1) theEschka method, (2) the bomb washing method, and (3) the high-temperaturecombustion method, and all are based on the combustion of the sulfur-containingmaterial to produce sulfate, which can be measured either gravimetrically or vol-umetrically. The Eschka method has distinct advantages in that the equipment
SULFUR 75is relatively simple and only the more convenient analytical techniques areemployed. However, methods involving combustion of the organic material in abomb have distinct advantages insofar as sulfur is not lost during the process,and such methods are particularly favored when the caloriﬁc value of the coal isalso required. The method of decomposition involves the Parr fusion procedurein the presence of sodium peroxide and oxygen at high pressures [300 to 450 psi(2.1 to 3.1 MPa)].In the Eschka method (ASTM D-3177; ISO 334; ISO 351), 1 g of the analysissample is thoroughly mixed with 3 g of Eschka mixture, which is a combina-tion of two parts by weight of light calcined magnesium oxide with one part ofanhydrous sodium carbonate. The combination of sample and Eschka mixture isplaced in a porcelain crucible (30 mL) and covered with another gram of Eschkamixture. The crucible is placed in a mufﬂe furnace, heated to a temperature of800 ± 25◦C (1472 ± 45◦F), and held at this temperature until oxidation of thesample is complete. The sulfur compounds evolved during combustion react withthe magnesium oxide (MgO) and sodium carbonate (Na2CO3) and under oxidiz-ing conditions are retained as magnesium sulfate (MgSO4) and sodium sulfate(Na2SO4). The sulfate in the residue is extracted and determined gravimetrically.In the bomb washing method, sulfur is determined in the washings from theoxygen bomb calorimeter following the calorimetric determination (ASTM D-2015 and ASTM D-3286; these standards have been discontinued but are stillused in many laboratories). After opening, the inside of the bomb is washedcarefully, and the washings are collected. After titration with standard base solu-tion to determine the acid correction for the heating value, the solution is heatedand treated with ammonium hydroxide (NH4OH) to precipitate iron ions as fer-ric oxide [Fe(OH)3]. After ﬁltering and heating, the sulfate is precipitated withbarium chloride (BaCl2) and determined gravimetrically.In the high-temperature combustion test method (ASTM D-4239, submethodsA, B, and C), a weighed sample is burned in a tube furnace at a minimum oper-ating temperature of 1350◦C (2462◦F) in a stream of oxygen to ensure completeoxidation of sulfur-containing components in the sample. Using these conditions,all sulfur-containing materials in the coal or coke are converted predominantlyto sulfur dioxide in a reproducible way. The amount of sulfur dioxide producedby burning the sample can be determined by the three alternative methods men-tioned above.In the acid–base titration method, the combustion gases are bubbled througha hydrogen peroxide solution in a gas absorption bulb. Sulfuric acid is producedby the reaction of sulfur dioxide with hydrogen peroxide and is determined bytitration with a standard base solution. Chlorine-containing species in the sampleyield hydrochloric acid in the hydrogen peroxide solution, which contributes toits total acidity. For accurate results, a correction must be made for the chlorinepresent in the sample (ASTM D-2361; ASTM D-4208; ISO 352; ISO 587).Appropriate standard reference materials should be used to calibrate commerciallyavailable sulfur analyzers to establish recovery factors or a calibration curve basedon the range of sulfur in the coal or coke samples being analyzed.
76 ULTIMATE ANALYSISIn the iodimetric titration procedure, the combustion gases are bubbled througha diluent solution containing pyridine, methanol, and water. This solution istitrated with a titrant containing iodine in a pyridine, methanol, and water solu-tion. In automated systems, the titrant is delivered automatically from a calibratedburette syringe and the endpoint detected amperometrically. The method is empir-ical, and standard reference materials with sulfur percentages in the range of thesamples to be analyzed should be used to calibrate the instrument before use.Alternative formulations for the diluent and titrant may be used in this methodto the extent that they can be demonstrated to yield equivalent results.The third method of measuring the sulfur dioxide in the combustion gases isby the absorption of infrared (IR) radiation. Moisture and particulates are ﬁrstremoved from the gas stream by traps ﬁlled with anhydrous magnesium perchlo-rate. The gas stream is then passed through an infrared absorption cell tunedto a frequency of radiation absorbed by sulfur dioxide. The infrared radiationabsorbed during combustion of the sample is proportional to the sulfur dioxidein the combustion gases and therefore to the sulfur in the sample. The method isempirical, and standard reference materials with sulfur percentages in the range ofthe samples to be analyzed should be used to calibrate the instrument before use.Some general problems associated with the determination of sulfur in coalare nonuniform distribution of pyrite particles, failure to convert all the sulfur tosulfate, and loss of sulfur as sulfur dioxide during the analysis. The nonuniformdistribution of pyrite necessitates the collection of many sample increments toensure that the gross sample is representative of the lot of coal in question. Pyriteparticles are both hard and heavy and have a tendency to segregate during thepreparation and handling of samples. Because the particles are harder, they aremore difﬁcult to crush and pulverize and tend to concentrate in the last portionof material that remains from these processes.In each of the methods discussed, sulfur is oxidized to sulfur dioxide duringthe analysis. Some sulfur dioxide may be lost unless the necessary precautionsare taken. In the Eschka method, a generous layer of Eschka mixture coveringthe fusion mixture helps prevent the loss of sulfur as sulfur dioxide. The mixturemust be heated gradually to guard against the production of sulfur dioxide at arate that is too high for it to be absorbed by the Eschka mixture. In the bombwashing method, the pressure of the bomb should be released slowly after thesample is burned in oxygen so that sulfur oxides will not be carried out of thebomb. In the high-temperature combustion methods, it is essential that the ﬂowof oxygen be sufﬁcient and that the rate of heating not be too high. A high rateof heating will lead to the evolution of combustion products, including sulfurdioxide, at a rate that is too rapid for complete absorption in the solutions or fordetection by the infrared cell.The gravimetric determination of sulfate can be and is most often used toﬁnish the Eschka and bomb washing methods. The most serious concern is thatthe barium sulfate precipitated may be extremely ﬁne and difﬁcult to ﬁlter. Thiscan be overcome by adding the barium chloride (BaCl2) rapidly to the hot solutionand stirring the mixture vigorously to obtain a barium sulfate (BaSO4) precipitate,
SULFUR 77which is easily ﬁltered out. In addition, heating and digestion for a lengthy periodimprove the ﬁlterability of the precipitate. After ﬁltering, the precipitate must bewashed several times with hot water to remove adsorbed materials that will causethe results to be too high.4.3.2 Determination of the Forms of SulfurAs noted above, sulfur occurs in coal in three forms (ASTM D-2492; ISO 157):(1) inorganic sulfur or sulfate sulfur [i.e., as sulfates of metals such as cal-cium sulfate (CaSO4)], (2) pyrite sulfur [i.e., as pyrite or marcasite (FeS2)], and(3) organic sulfur (i.e., as sulfur combined organically in the coal). Organic sul-fur and pyrites account for almost all the sulfur in coal. Sulfate sulfur is usuallyless than 0.1%, except in weathered coal containing an appreciable amount ofpyrites. The pyrite sulfur content varies considerably more than does the organicsulfur content and is of more interest because it is the form that can most easilybe removed from coal by current preparation practices.The methods used for the determination of the various forms of sulfur in coalare based on the fact that sulfate sulfur is soluble in dilute hydrochloric acidsolution, whereas pyrite and organic sulfur are not attacked. In addition, dilutenitric acid dissolves sulfate and pyrite sulfur quantitatively and attacks organicsulfur only slightly. Pyrite sulfur, however, is determined accurately by notingthe quantity of iron extracted by dilute hydrochloric acid and subtracting thisfrom the iron extracted by nitric acid, the difference being the iron present aspyrite iron (FeS2), from which the equivalent quantity of pyrite sulfur can becalculated. Sulfate sulfur and pyrite sulfur may therefore be determined on theone sample of coal, but since the sulfate sulfur determination is rather tedious,it is customary to use separate samples for each determination. Organic sulfuris then obtained by subtracting the combined percentages of sulfate sulfur andpyrite sulfur from the total sulfur determined by the Eschka method.In the method for determining the forms of sulfur in coal (ASTM D-2492; ISO157), the sulfate and pyrite sulfur are determined directly, and the organic sulfuris taken as the difference between the total sulfur and the sum of the sulfate andpyrite sulfur.In the determination of sulfate, 2 to 5 g of the analysis sample is mixed withHCl (2 volumes concentrated HCl + 3 volumes of water), and the mixture isgently boiled for 30 minutes. After ﬁltering and washing, the undissolved coalmay be retained for the determination of pyrite sulfur, or it may be discardedand a fresh sample used for pyrite sulfur. Saturated bromine water is added tothe ﬁltrate to oxidize all sulfur forms to sulfate ions and ferrous ions to ferricions. After boiling to remove excess bromine, the iron is precipitated with excessammonia and ﬁltered. This precipitate must be retained for the determinationof nonpyrite iron if a fresh sample of coal was used for the determination ofthe pyrite iron. The sulfate is then precipitated with BaCl2, and the BaSO4 isdetermined gravimetrically.Either the residue from the sulfate determination or a fresh 1-g sample isused for the determination of pyrite sulfur content. The sample is added to dilute
78 ULTIMATE ANALYSISnitric acid and the mixture boiled gently for 30 minutes or allowed to standovernight. This treatment oxidizes iron species to iron(III) and inorganic sulfurcompounds to sulfate. The mixture is then ﬁltered, and the ﬁltrate is saved for thedetermination of iron by atomic absorption spectrophotometry or by a titrationprocedure. If iron is to be determined by the atomic absorption method, no furtherwork is done on the ﬁltrate other than to dilute it to an appropriate volume beforethe determination. If a titration method is to be used for the determination of iron,the ﬁltrate is treated with 30% H2O2 to destroy any coloration arising from thecoal. The iron is then precipitated, ﬁltered, and washed. The precipitate is thendissolved in HCl, and the iron determined by titration with either potassiumdichromate (K2Cr2O7) or potassium permanganate (KMnO4).If a new sample is used for the determination of pyrite iron, the iron determinedby these procedures represents the combination of the pyrite and nonpyrite iron.The amount of nonpyrite iron must then be determined separately and subtractedfrom the amount determined. If the residue from the sulfate determination wasused, the iron determined by the foregoing procedures represents the pyrite iron.Once the correct value for the pyrite iron is determined, the pyrite sulfur iscalculated using the following expression:% pyrite sulfur = % pyrite iron × 2 ×32.0655.85(4.2)where 2 × 32.06/55.85 is the ratio of sulfur to iron in pyrite.Some difﬁculties encountered in determining the amounts of the various formsof sulfur in coal are adsorption of other materials on barium sulfate (BaSO4)when it is precipitated, inability to extract all the pyrite sulfur from the coalduring the extraction process, and possible oxidation of pyrite sulfur to sulfatein the pulverization and storage of the coal sample. Both the adsorption of othermaterials on barium sulfate and oxidation of pyrite sulfur lead to high valuesfor the sulfate sulfur. Iron ions (Fe2+) are readily adsorbed on barium sulfate,which could be particularly objectionable for coals containing large amountsof nonpyrite iron. Removal of the iron by precipitation and ﬁltration beforethe precipitation of barium sulfate minimizes adsorption of the iron. Inadequatepulverization and mixing of the sample appear to be the major causes of theincomplete extraction of pyrite sulfur from coal. A very small amount of organicsulfur may also be extracted with the pyrite sulfur. For this reason, the amountof pyrite iron extracted is used as a measure of the pyrite sulfur. To controlthe oxidation of pyrite sulfur to sulfates, exposure of the coal sample to theatmosphere at elevated temperatures should be avoided, and the sample shouldbe analyzed as soon as possible.X-ray ﬂuorescence has been used extensively for determining total sulfur incoal. The economy and speed of such x-ray ﬂuorescence methods when used formultiple determinations (e.g., Al, Si, Ca, Mg, Fie, K, Ti, P, and S) in the sameprepared coal sample are probably unsurpassed by any other method.A neutron sulfur meter was developed for continuous monitoring of the sul-fur content of coal from a preparation plant. Neutrons from a radioactive source
OXYGEN 79produced thermal neutrons within the sample, which produced prompt gamma-ray emissions when captured by atoms in the coal. The gamma-ray energiescharacteristic of sulfur were measured by a sodium iodide crystal and associ-ated electronic equipment. Several methods to eliminate interferences from otherelements, moisture, and bulk density were evaluated. Results from the neutronsulfur meter for total sulfur in coal agreed closely with chemical analyses, andthe method is precise (±0.05% absolute), rapid, and suitable for online sulfurdetermination.High-resolution x-ray spectroscopy was employed successfully to determinethe chemical state of sulfur in coal. Fluorescent x-rays from pressed coal pow-ders, excited with x-rays from a chromium target tube, were analyzed using agermanium crystal. The sulfur Ka radiation increased with increasing oxidationnumber, allowing quantitative determinations of the sulfur types.Another method of direct determination of organic sulfur is to subject a small(20- to 30-mg) sample of <200-mesh coal to low-temperature ashing 1 to 3 hoursand to collect the sulfur oxides evolved in a cold trap. They are then absorbedin hydrogen peroxide (H2O2) and determined chromatographically.Mossbauer spectrometry is also useful to identify multiple iron species in coaland charred residues without using a concentration step. The results indicatethat heat treatment of any kind, even at temperatures as low as 175◦C (347◦F),changes the nature of the iron species in coal. Furthermore, some kind of anassociation between the pyrite (FeS2) in whole coal and the organic matrix wasindicated. The pyrite also appeared to be altered when the coal was heated to175◦C (347◦F).4.3.3 Data Handling and InterpretationThe principal use of forms of sulfur data is in connection with the cleaning ofcoal. Within certain limits, pyrite sulfur can be removed from coal by gravityseparation methods, whereas organic sulfur cannot. Pyrite sulfur content cantherefore be used to predict how much sulfur can be removed from the coal andto evaluate cleaning processes. If the pyrite sulfur occurs in layers, it can usuallybe removed efﬁciently. If it occurs as ﬁne crystals dispersed throughout the coal,its removal is very difﬁcult.Other uses of forms of sulfur data are the inclusion of the pyrite sulfur valuein the formula for the estimation of oxygen by difference and as a possible meansof predicting the extent of weathering of coal. The sulfate concentration increasesupon weathering, so the sulfate sulfur value could be used as an indication ofthe extent of weathering of coal.4.4 OXYGENOxygen occurs in both the organic and inorganic portions of coal. In the organicportion, oxygen is present in hydroxyl (–OH), usually phenol groups, carboxylgroups (CO2H), methoxyl groups (–OCH3), and carbonyl groups (=C=O). In
80 ULTIMATE ANALYSISlow-rank coal, the hydroxyl oxygen averages about 6 to 9%, whereas high-rankcoals contain less than 1%. The percentages of oxygen in carbonyl, methoxyl,and carboxyl groups average from a few percent in low rank and brown coalto almost no measurable value in high-rank coal. The inorganic materials incoal that contain oxygen are the various forms of moisture, silicates, carbonates,oxides, and sulfates. The silicates are primarily aluminum silicates found in theshalelike portions. Most of the carbonate is calcium carbonate (CaCO3), theoxides are mainly iron oxides (FeO and Fe2O3), and the sulfates are calcium andiron (CaSO4 and FeSO4).4.4.1 Test Method ProtocolsFor many years, no satisfactory method existed for the direct determination ofoxygen in coal. In practice, in the expression of the ultimate analysis it is cus-tomary to deduct from 100.0 the sum of the percentages of moisture, ash, carbon,hydrogen, nitrogen, and sulfur (ASTM D-3176):% oxygen = 100 − (%C + %H + %N + %Sorganic) (4.3)The resulting ﬁgure for oxygen is therefore burdened with the accumulation of allthe experimental errors involved in the determinations of the other constituentsthat form part of the equation. Consequently, the oxygen content was, and stillis, of a low order of accuracy. For this reason, oxygen determined by differenceshould not be designated percent oxygen but percent oxygen by difference.The most widely used procedure for oxygen determination consists of pyrolyz-ing coal in the presence of nitrogen and subsequent passage of the products overhot (1100◦C, 2012◦F) carbon or platinized carbon (ISO, 1994). The oxygen inthe volatile products is thereby converted to carbon monoxide, which can bedetermined by a variety of techniques (Gluskoter et al., 1981; Frigge, 1984).For example, the carbon monoxide can be oxidized to carbon dioxide, usu-ally with iodine pentoxide, which releases free iodine. The iodine released canbe determined titrimetrically, or the carbon dioxide produced can be absorbedand determined gravimetrically to calculate the amount of oxygen in the origi-nal samples.However, the various sources of oxygen in coal, such as the oxygen in themoisture and water of hydration of mineral matter, the oxygen in carbonates,and the oxygen in silicates and other inorganic compounds, in addition to theoxygen in the organic matter, all offer hurdles in producing data that are beyondquestion. The original procedure has been modiﬁed in several ways to reduce thecontribution made by some of these oxygen sources to the determined oxygenvalue. Thorough drying in a nitrogen atmosphere before pyrolysis of the sampleminimizes the effect of moisture, and much of the mineral matter is removedby a speciﬁc gravity separation or chemical treatment with hydrochloric andhydroﬂuoric acid. The reduction of mineral matter minimizes the contributionthat the water of hydration and the inorganic compounds, such as carbonates,silicates, oxides, and sulfates, make to the oxygen value that is determined. After
OXYGEN 81all the pretreatment steps are taken to remove moisture and mineral matter, theoxygen value obtained by this method is essentially a measure of the oxygencontained in the organic matter in coal.Several other methods for the direct determination of oxygen have met withsome success when applied to coal and therefore deserve mention here, becauseit is conceivable that at some future date one of these methods (or a modiﬁca-tion thereof) could ﬁnd approval as a recognized standard method for the directdetermination of oxygen in coal.An oxidation method that has been applied to coal involves the combustion ofa weighed amount of coal with a speciﬁc quantity of oxygen. The oxygen in thecoal is determined by deducting the added quantity of oxygen from the sum ofthe residual oxygen and the oxygen of the oxidation products. The disadvantagesof the method arise because of the difﬁculties associated with the accurate mea-surement of the substantial volume of oxygen used and the quantity and quality(i.e., composition) of the combustion products.Another method for the determination of oxygen in coal involves reductionof the coal by pyrolysis in the presence of hydrogen, whereupon the oxygen isconverted catalytically to water. However, the procedure is relatively complexand the catalyst may be poisoned by sulfur and by chlorine.In the neutron activation method (Volborth, 1979a,b; Volborth et al., 1987;Mahajan, 1985), as illustrated by the reaction16O + neutron = 16N + proton (4.4)the concentration of oxygen is determined by measuring the radiation from thesample. The method is nondestructive and rapid, but if only the organic oxygenis to be determined, the sample must ﬁrst be demineralized.Because oxygen in coal includes both oxygen in organic matter and inorganicoxygen from mineral matter and moisture, demineralization or ﬂoat–sink clean-ing of coal is usually employed to remove inorganic oxygen. Using a modiﬁedmethod (ISO 602; ISO, 1994), the results of the direct determination of oxygenin untreated coals showed signiﬁcant variations from oxygen values obtained bythe difference method. The differences were caused primarily by sulfur trioxidebeing retained in the ash, sulfur in the pyrite form in the whole coal, and smallquantities of inorganic oxygen. Much closer agreement was obtained when ashvalues used for calculation of oxygen by difference were corrected to a betterapproximation of mineral matter:corrected ash = ashdetermlned − SO3ash (4.5)Pyrite sulfur in whole coal is added to the ash value, organic sulfur is added in theultimate analysis as part of the coal substance, and CO from carbonates is addedto total carbon and oxygen values. Demineralized coals gave the best results fororganic oxygen; values from untreated coals were usually higher because theyincluded inorganic oxygen.
82 ULTIMATE ANALYSISThe use of gas chromatography to determine oxygen in coal is considerablyfaster than the methods just described. The oxygen produced from coal pyroly-sis in a vacuum was converted to carbon monoxide catalytically, and the totalquantity of gas was measured. Gas chromatography was then used to measurethe concentration of carbon monoxide in the gas.A method employing reduction fusion using radio-frequency heating of coalhas been reported for the determination of oxygen in coal. An induction furnacewas used to heat an iron–tin bath in a graphite crucible supported in a bed ofcarbon black powder that was contained in a silica thimble. All were enclosed ina reaction tube through which argon carrier gas ﬂowed. Pyrolysis products froma sealed coal sample (10 mg) dropped into the bath were puriﬁed, and oxygenwas converted to carbon dioxide that was absorbed and weighed. Satisfactoryresults were obtained for organic oxygen in demineralized coal. For untreatedcoal, satisfactory results were obtained when a range of correction techniques foroxygen was applied to coals containing more than 5% ash.4.4.2 Data Handling and InterpretationWhen the oxygen value is estimated by subtracting from 100 the percentagesdetermined for all other constituents, the errors in the values determined arereﬂected in the oxygen value estimated. These errors may be partially compen-sating, or they may be additive. It is important that accurate determinations bemade and appropriate corrections for overlapping values, especially hydrogen, becalculated. Thus,O = 100 − (C + H + N + S + ash) (4.6)All values are expressed as percentages and C is the as-determined carbon(ASTM D-3178), H is the as-determined hydrogen (ASTM D-3178), N is theas-determined nitrogen (ASTM D-3179), S is the as-determined sulfur (ASTMD-3177; ASTM D-4239), and “ash” is the as-determined ash (ASTM D-3174).All the values above pertain to those obtained from the analysis sample. The as-determined value for carbon represents both organic and carbonate carbon. Theas-determined value for hydrogen represents the organic hydrogen, the hydrogenin the residual moisture, and the hydrogen in the water of hydration of mineralmatter. The sulfur value is the total sulfur in coal and represents that which iscontained in the organic matter, pyrites, and sulfates. Ash is mostly metal oxidesand silicon oxide. The estimated value of the oxygen therefore includes the oxy-gen contained in the organic matter, in the moisture, and in the mineral matter,except that which is combined with metals in coal ash.A rough estimate of the oxygen contained in the organic matter in coal canbe obtained by correcting the oxygen value obtained by equation (4.6) for theoxygen in residual moisture and water of hydration of mineral matter. Addingthis correction to the sum subtracted from 100 gives the following expression:Ox = 100 − [C + H + N + S + ash + 89(H2O + H2O of hydration)] (4.7)
OXYGEN 83where H2O is the as-determined residual moisture (ASTM D-3173) and the H2Oof hydration is 8.0% of ash.Several improvements in the estimation of organic oxygen can be made whenanalytical data are available. Values for chlorine, carbon dioxide, pyrite sulfur,and sulfur in coal ash are helpful in improving the estimation. Failure to includethe chlorine value in the sum subtracted from 100 leads to a high value for theorganic oxygen. This oxygen value should also be reduced for the oxygen presentin the carbon dioxide that is associated with the mineral matter.The inclusion of both total sulfur and ash in the sum that is subtracted from100% in estimating the oxygen content of coal lowers the oxygen value, sincepart of the sulfur may be retained in the ash. The sulfur that is retained is thereforecounted twice in the sum for subtraction. Correcting the coal ash for the sulfurtrioxide (SO3) present compensates for this error. Similarly, the coal ash shouldbe corrected for any ferric oxide (Fe2O3) that results from the heating of pyrite(FeS2) in air, as is done in the ashing process. In the ashing process, three oxygenatoms replace four sulfur atoms:4FeS2 + 11O2 → 2Fe2O3 + 8SO2 (4.8)On a weight basis, 48 parts of oxygen replace 128 parts of sulfur. This oxy-gen is from an external source and not from the coal itself. Since this oxygencontributes to the weight of the ash, correction for the pyrite sulfur value isnecessary. The pyrite sulfur that is replaced is accounted for in the total sulfurvalue. When the values are available to make these corrections, a good estimatecan be made of the percentage of oxygen in the organic or combustible portionof coal:O = 100 − [C + H + N + S + Cl + (ash − %Sp − SO3ash)+ 89(H2O + H2Ohydration) + 3244CO2] (4.9)Chlorine is the as-determined chlorine (ASTM D-2361; ASTM D-4208), Sp is theas-determined pyrite sulfur (ASTM D-2492), SO3ash is the as-determined sulfate(sulfur trioxide, SO3) in ash (ASTM D-1757), and CO2 is the as-determinedcarbon dioxide in coal (ASTM D-1756). All other terms are as given in theearlier formulas, and all values are expressed as percentages.If the oxygen is determined directly, using the method discussed previously inwhich the moisture and mineral matter are removed from the sample before actualoxygen determination, the oxygen value in this case represents that contained inthe organic matter. In calculating heat balances for boiler efﬁciency studies, it isimportant that an accurate value of the combustible material in coal be obtained.Thus, a correction for the oxygen content of the organic matter of coal should bemade. Of course, corrections to the carbon and hydrogen values for the amountof these elements found in the moisture and inorganic constituents of coal shouldalso be made. Oxygen data are used for determining the suitability of coalsfor coking, liquefaction, or gasiﬁcation processes. In general, coals with a high
84 ULTIMATE ANALYSISoxygen content are unsuitable for coking but may be more reactive and thuseasier to gasify or liquefy.4.5 CHLORINEChlorine occurs in coal (Chakrabarti, 1978, 1982; Hower et al., 1992) and isbelieved to be a factor not only in fouling problems but also in corrosion prob-lems (Canﬁeld et al., 1979; Slack, 1981). The chlorine content of coal is normallylow, usually only a few tenths of a percent or less. It occurs predominantly assodium, potassium, and calcium chlorides, with magnesium and iron chloridespresent in some coals. There is evidence that chlorine may also be combinedwith the organic matter in coal.4.5.1 Test Method ProtocolsMethods of converting the chlorine in coal into a form suitable for its analyticaldetermination include combusting the sample, with or without Eschka mixture, inan oxygen bomb and heating with Eschka mixture in an oxidizing atmosphere.Eschka mixture is a combination of two parts by weight of magnesium oxideand one part of anhydrous sodium carbonate. There are two standard methods ofdetermining chlorine in coal (ASTM D-2361; ASTM D-4208).The ﬁrst method (ASTM D-2361) offers a choice of two procedures for com-busting the coal sample. In the bomb combustion procedure, the oxygen bombused is the same as, or very similar to, that used in determination of the caloriﬁcvalue (ASTM D-2015; ASTM D-3286).In the ﬁrst procedure (ASTM D-2361), a weighed sample (approximately 1 g)is mixed with a weight amount (approximately 1 g) of the Eschka mixture andplaced in a crucible inside an oxygen bomb. An ammonium carbonate solution isadded to the bomb to trap the chloride-containing species produced in the com-bustion. After charging with oxygen to 25 atm, the bomb is ﬁred and allowed tostand in the calorimeter water for at least 10 minutes. The pressure on the bomb isthen released slowly, the bomb is disassembled, and all parts of the bomb interiorare washed with hot water. The washings are collected in a beaker and acidiﬁedwith nitric acid. The amount of chloride in the solution is then determined byeither a modiﬁed Volhard or by a potentiometric titration with silver nitrate solu-tion. In the second procedure (ASTM D-2361), 1 g of the coal analysis sample ismixed with 3 g of Eschka mixture in a suitable crucible. This mixture is coveredwith an additional 2 g of Eschka mixture to ensure that no chlorine is lost duringcombustion. The mixture is then ignited gradually in a mufﬂe furnace by raisingthe temperature to 675 ± 25◦C within 1 hour. This temperature is maintained for1 hour before the cooling and washing of the incinerated mixture with hot waterinto a beaker. The contents of the beaker are acidiﬁed with nitric acid, and thechloride is determined as in the procedure described previously.In second test method (ASTM D-4208), 1 g of the analysis sample of coalis placed in a crucible inside an oxygen bomb. A sodium carbonate solution
CHLORINE 85is added to the bomb to trap the chloride-containing species produced. Aftercharging with oxygen to 25 atm, the bomb is ﬁred and allowed to stand in thecalorimeter water for at least 15 minutes. After the pressure is released veryslowly, the bomb is disassembled, and all parts of the bomb interior are washedwith water. The washings are collected, an ionic strength adjuster (sodium nitrate,NaNO3) is added, and the chloride is determined with an ion-selective electrodeby the standard addition method.In both methods it is possible to lose some of the chlorine during combustionunless necessary precautions are taken. Thoroughly mixing the coal sample withEschka mixture and covering this carefully with additional Eschka mixture min-imizes the loss of chlorine. In bomb combustion methods, the ammonium andsodium carbonate solutions in the bomb are used to absorb the chlorine as it isreleased in the combustion. The 10- and 15-minute waiting periods and the slowrelease of pressure on the bomb help to prevent the loss of chlorine as well.A modiﬁcation of the oxygen bomb combustion method (ASTM D-2361) forthe determination of chlorine consisted of acidifying a solution of the adsorbedcombustion products and titrating the chlorine potentiometrically. A potentio-metric titration was also tried for the determination of chlorine by the oxygenﬂask method. Combustion products, including chlorine, were absorbed in sodiumhydroxide (NaOH), and the chloride was measured using silver–silver chlo-ride electrodes. Although there was no statistical difference in results obtainedfrom potentiometric titration and the Eschka procedure, the latter wasmore precise.There is also a test method (ASTM E-256) for the determination of chlorinein organic compounds by sodium peroxide bomb ignition that is also worthy ofreference. The method is intended for application to samples of organic materialscontaining more than 0.5% chlorine, and the assumption is that halogens otherthan chlorine will not be present.4.5.2 Data Handling and InterpretationThe chlorine in coal and in the products derived from coal is known to con-tribute signiﬁcantly to corrosion of the coal-handling and coal-processing equip-ment. Since the corrosion of this equipment is the result of several causes, onebeing the chlorine content of coal, it is difﬁcult to predict the degree of corro-sion within a given time frame. It is equally difﬁcult to predict the degree towhich the chlorine content contributes to the corrosion, other than the generalprediction that the higher the chlorine content, the greater the chances for cor-rosion of the equipment. As a general rule, coal with a high chlorine content isnot desirable.Chlorine data are used in ultimate analysis to improve the estimate of oxygenby difference. The chlorine value is included in the sum of the items determined,which, when subtracted from 100, gives an estimate of the oxygen content of coal.Although the validity of the analytical data is uncertain, a generally acceptedfouling classiﬁcation of coal, according to total chlorine content (ASTM D-2361;ISO 352; ISO 587), is as follows:
86 ULTIMATE ANALYSISTotal PercentChlorine in Coal Fouling Type<0.2 Low0.2–0.3 Medium0.3–0.5 High>0.5 SevereIn terms of corrosion, the occurrence of chlorine in coal leads to the formationof hydrogen chloride, and the condensation of water containing hydrogen chloride(hydrochloric acid) on the cooler parts of combustion equipment can lead tosevere corrosion of the metal surfaces.4.6 MERCURYMercury has been identiﬁed as a very dangerous environmental contaminant,largely by reason of the process of concentration in the food chain. Thus, thepresence of mercury in coal is an extremely sensitive issue. The possible emissionof mercury that may be found in coal is an environmental concern.The test for total mercury (ASTM D-3684; ISO 15237) involves combusting aweighed sample in an oxygen bomb with dilute nitric acid absorbing the mercuryvapors. The bomb is rinsed into a reduction vessel with dilute nitric acid, and themercury is determined by the ﬂameless cold vapor atomic absorption technique.Mercury and mercury salts can be volatilized at low temperatures. Precautionsagainst inadvertent mercury loss should be taken when using this method. Whencoal samples are burned according to this procedure, provided that sample prepa-ration in is accord with the standard procedure (ASTM D-2013), the total mercuryis quantitatively retained and is representative of concentrations in the whole coal.Caution is also advised in use of the bomb, considering the chemicals requiredfor the test method.Another test method for the determination of mercury in coal (ASTM D-6414)involves (method A) solubilizing of the mercury in the sample by heating thesample at a speciﬁed temperature in a mixture of nitric and hydrochloric acids.The acid solutions produced are transferred into a vessel in which the mercuryis reduced to elemental mercury. The mercury vapor is determined by ﬂamelesscold-vapor atomic absorption spectroscopy. An alternative method (method B)involved solubilization of the mercury by heating the sample in a mixture ofnitric acid and sulfuric acid with vanadium pentoxide. The acid solution is thentransferred into a vessel in which the mercury is reduced to elemental mercury.The mercury content is determined by ﬂameless cold-vapor atomic absorptionspectroscopy. However, mercury and mercury salts can be volatilized at lowtemperatures, and precautions against inadvertent mercury loss should be takenwhen using this method.The determination of mercury in coal, and in coal combustion residues, canalso be accomplished by controlled heating of the sample in oxygen (ASTM
OTHER CONSTITUENTS 87D-6722). The sample is heated to dryness and then decomposed thermally andchemically. The decomposition products are carried by ﬂowing oxygen to the cat-alytic section of the furnace, where oxidation is completed and halogens as wellas nitrogen and sulfur oxides are trapped. The remaining decomposition prod-ucts are carried to a gold amalgamator that traps mercury selectively. After thesystem is ﬂushed with oxygen to remove any remaining decomposition products,the amalgamator is heated rapidly, releasing mercury vapor. Flowing oxygen car-ries the mercury vapor through absorbance cells positioned in the light path of asingle-wavelength atomic absorption spectrophotometer. Absorbance peak heightor peak area, as a function of mercury concentration, is measured at 253.7 nm.As before, precautions must be taken against loss of mercury and mercury saltsthat are volatile at low temperatures.4.7 OTHER CONSTITUENTSSeveral of the minor components of coal are of importance, because of the quan-tity present on occasion, but more so in some cases by virtue of the specialproperties they possess which are undesirable when the coal is used for certainpurposes. For example, to arrive at a correct ﬁgure for the combustible carbonin coal, it is necessary to apply a correction for the quantity of carbonate asso-ciated with the sample. Combustion analyses determine only the total carbon.Again, coking coals should have low phosphorus content, and anthracites usedfor malting should contain only very small quantities of arsenic, so that the deter-mination of these elements becomes necessary in certain cases. Since both arefound normally in small amounts, they are not included in the general statementof the ultimate analysis but are reported separately.4.7.1 Carbon DioxideMost coals contain small amounts of mineral carbonates made up primarily ofcalcium carbonate and to a lesser extent ferrous and other metal carbonates. Somecoals contain a comparatively large amount of the inorganic carbonates, and thedetermination of carbon dioxide content is required in estimating the mineralmatter content of these high-carbonate coals. Indeed, it is necessary to have aknowledge of the carbonate content of coal to correct the carbon ﬁgure and since,without resorting to very elaborate analyses, it would be impossible to expressthe carbonate content as deﬁnite quantities of calcium carbonate, magnesiumcarbonate, and so on, it is customary, and sufﬁcient for all analytical purposes,to express it simply in terms of carbon dioxide.One particular test method (ASTM D-1756) covers the determination of carbondioxide in coal in any form, such as mineral carbonate, from which carbon dioxideis released by action of mineral acids (e.g., hydrochloric acid). The method canbe applied to high- and low-carbonate coals. The determination of carbon dioxideis made by decomposing with acid a weighed quantity of the sample in a closedsystem and absorbing the carbon dioxide in an absorbent (e.g., such as sodium
88 ULTIMATE ANALYSIShydroxide, NaOH, or potassium hydroxide, KOH). The increase in weight of theabsorbent is a measure of the carbon dioxide in the sample, which can be usedto calculate the amount of mineral carbonates in the coal.Due to the small amount of carbon dioxide in coal and the difﬁculty of mea-suring accurately the carbon dioxide that is liberated, some strict requirementshave been set for the construction and design of the apparatus to be used (ASTMD-1756). The apparatus must contain an airﬂow meter and purifying train, areaction unit ﬁtted with a separator funnel and water-cooled condenser, a unitfor removing interfering gases, and an absorber. The air-purifying train removesall carbon dioxide, and the water-cooled condenser removes moisture before itcan enter the absorption train. Acid-forming gases, such as sulfur dioxide andhydrogen sulﬁde, and halogen acids are produced in the reaction and must beremoved before entering the CO2 absorber. Otherwise, they will be weighed asabsorbed and measured as carbon dioxide. Anhydrous copper sulfate on pumiceor granular silver sulfate is positioned in the absorption train to remove theseinterfering gases from the airstream before it enters the CO2 absorber. The entiresystem must be gastight to prevent error, and a time schedule is speciﬁed toensure repeatability and reproducibility.Another option (ASTM D-6316) involved determination of the total, com-bustible, and carbonate carbon remaining in the solid by-products of combustionfrom boiler furnaces and similar reactors, including ash, ﬂy ash, char, slag, andsimilar materials. The determination of total carbon is made by the oxidative ther-mal decomposition of a weighed quantity of sample in a closed system, and aftercomplete oxidation and puriﬁcation of the resulting gaseous products, measure-ment of the carbon dioxide produced by one of several methods. The evolvedcarbon dioxide is ﬁxed on an absorption train and is measured quantitativelyby weighing the absorbent (ASTM D-3178). The carbon dioxide is measuredquantitatively by an electronic detection system calibrated against an appropriatereference standard (ASTM D-5373).This test method is intended for the use of industry to determine the perfor-mance of boiler furnaces and similar combustion reactors and aid in determiningthe quality of the solid residue from combustion. Any of several methods can beused to determine the total carbon content combined with any of several methodsto determine carbonate carbon, and the calculation, by difference, of the com-bustible carbon remaining in the sample. Alternatively, this test method appliesto the determination of total carbon remaining in a material after acidiﬁcationwith strong acid to evolve carbonate carbon.4.7.2 Arsenic and SeleniumArsenic and selenium occur in coal to the extent of several parts per millionand on combustion of the coal, varying quantities of these elements are releasedor retained in the ash, depending largely on the conditions under which thecombustion takes place and on the nature of the coal ash.Arsenic and selenium are determined (ASTM D-4606) by mixing a weighedsample with Eschka mixture and igniting at 750◦C (1382◦F). The mixture is
REFERENCES 89dissolved in hydrochloric acid and the gaseous hydride of each element is gen-erated from the appropriate oxidation state and determined by atomic absorptionspectrophotometry. The method permits measurement of the total arsenic andselenium content of coal for the purpose of evaluating these elements where theycan be of concern, for example, in coal combustion. When coal samples areprepared for analysis in accordance with standard procedure (ASTM D-2013),the arsenic and selenium are quantitatively retained and are representative of thetotal amounts in the coal.REFERENCESAhmed, S. M., and Whalley, B. J. P. 1978. In Analytical Methods for Coal and CoalProducts, Vol. 1, C. Karr, Jr. (Editor). Academic Press, San Diego, CA, Chap. 8.ASTM. 2004. Annual Book of ASTM Standards, Vol. 05.06. American Society for Testingand Materials, West Conshohocken, PA. Speciﬁcally:ASTM D-1756. Standard Test Method for Determination as Carbon Dioxide of Car-bonate Carbon in Coal.ASTM D-1757. Standard Test Method for Sulfate Sulfur in Ash from Coal and Coke.ASTM D-2013. Standard Practice of Preparing Coal Samples for Analysis.ASTM D-2015. Standard Test Method for Gross Caloriﬁc Value of Coal and Coke bythe Adiabatic Bomb Calorimeter.ASTM D-2361. Standard Test Method for Chlorine in Coal.ASTM D-2492. Standard Test Method for Forms of Sulfur in Coal.ASTM D-3173. Standard Test Method for Moisture in the Analysis Sample of Coaland Coke.ASTM D-3174. Standard Test Method for Ash in the Analysis Sample of Coal andCoke from Coal.ASTM D-3176. Standard Practice for Ultimate Analysis of Coal and Coke.ASTM D-3177. Standard Test Methods for Total Sulfur in the Analysis Sample ofCoal and Coke.ASTM D-3178. Standard Test Methods for Carbon and Hydrogen in the AnalysisSample of Coal and Coke.ASTM D-3179. Standard Test Methods for Nitrogen in the Analysis Sample of Coaland Coke.ASTM D-3286. Standard Test Method for Gross Caloriﬁc Value of Coal and Coke bythe Isoperibol Bomb Calorimeter.ASTM D-3684. Standard Test Method for Total Mercury in Coal by the Oxygen BombCombustion/Atomic Absorption Method.ASTM D-4208. Standard Test Method for Total Chlorine in Coal by the Oxygen BombCombustion/Ion Selective Electrode Method.ASTM D-4239. Standard Test Methods for Sulfur in the Analysis Sample of Coal andCoke Using High Temperature Tube Furnace Combustion Methods.ASTM D-4606. Standard Test Method for Determination of Arsenic and Selenium inCoal by the Hydride Generation/Atomic Absorption Method.
90 ULTIMATE ANALYSISASTM D-5373. Standard Test Methods for Instrumental Determination of Carbon,Hydrogen, and Nitrogen in Laboratory Samples of Coal and Coke.ASTM D-6316. Standard Test Method for Determination of Total, Combustible andCarbonate Carbon in Solid Residues from Coal and Coke.ASTM D-6414. Standard Test Method for Total Mercury in Coal and Coal CombustionResidues by Acid Extraction or Wet Oxidation/Cold Vapor Atomic Absorption.ASTM D-6722. Standard Test Method for Total Mercury in Coal and Coal CombustionResidues by Direct Combustion Analysis.ASTM E-256. Standard Test Method for Chlorine in Organic Compounds by SodiumPeroxide Bomb Ignition.Attar, A. 1979. In Analytical Methods for Coal and Coal Products, Vol. 3, C. Karr, Jr.(Editor). Academic Press, San Diego, CA, Chap. 56.BS. 2003. Methods for Analysis and Testing of Coal and Coke. BS 1016. British StandardsAssociation, London.Canﬁeld, D. R., Ibarra, S., and McCoy, J. D. 1979. Hydrocarbon Process., 58(7):203.Chakrabarti, J. N. 1978a. In Analytical Methods for Coal and Coal Products, Vol. 1,C. Karr, Jr. (Editor). Academic Press, San Diego, CA, Chap. 9.Chakrabarti, J. N. 1978b. In Analytical Methods for Coal and Coal Products, Vol. 1,C. Karr, Jr. (Editor). Academic Press, San Diego, CA, Chap. 10.Chakrabarti, J. N. 1982. In Coal and Coal Products: Analytical Characterization Tech-niques, E. L. Fuller Jr. (Editor). Symposium Series 205. American Chemical Society,Washington, DC, Chap. 8.Frigge, J. 1984. Erdoel Kohle Erdgas Petrochem., 37:267.Gluskoter, H. J., Shimp, N. F., and Ruch, R. R. 1981. In Chemistry of Coal Utilization,2nd Suppl. Vol., M. A. Elliott (Editor). Wiley, Hoboken, NJ, Chap. 7.Gorbaty, M. L., Kelemen, S. R., George, G. N., and Kwiatek, P. J. 1992. Fuel, 71:1255.Hower, J. C., Riley, J. T., Thomas, G. A., and Griswold, T. B. 1992. J. Coal Qual.,10:152.DIN. 2004. Standards for Fuel Analysis. Deutsches Institut f¨ur Normung, Berlin. Specif-ically:DIN 15722. Testing of Solid Fuels; Determination of Nitrogen Content; Dumas Method.DIN 51722. Testing of Solid Fuels; Determination of Nitrogen Content; Semi-MicroKjeldahl Method.ISO. 1994. Hard Coal—Determination of Oxygen Content. International Organization forStandardization, Geneva, Switzerland.ISO. 2003. Standard Test Methods for Coal Analysis. International Organization forStandardization, Geneva, Switzerland. Speciﬁcally:ISO 157. Determination of Forms of Sulfur.ISO 333. Determination of Nitrogen: Semi-micro Kjeldahl Method.ISO 334. Determination of Total Sulfur: Eschka Method.ISO 351. Determination of Total Sulfur: High Temperature Combustion Method.ISO 352. Determination of Chlorine: High Temperature Combustion Method.ISO 587. Determination of Chlorine Using Eschka Mixture.ISO 602. Coal: Determination of Mineral Matter.
REFERENCES 91ISO 609. Determination of Carbon and Hydrogen: High Temperature CombustionMethod.ISO 625. 2003. Determination of Carbon and Hydrogen: Liebig Method.ISO 15237. 2003. Determination of Total Mercury Content of Coal.Kuhn, J. K. 1977. In Coal Desulfurization, T. D. Wheelock (Editor). Symposium Series64. American Chemical Society, Washington, DC, p. 16.Raymond, R., Jr. 1982. In Coal and Coal Products: Analytical Characterization Tech-niques, E. L. Fuller, Jr. (Editor). Symposium Series 205. American Chemical Society,Washington, DC, Chap. 9.Slack, A. V. 1981. In Chemistry of Coal Utilization, 2nd Suppl. Vol., M. A. Elliott (Edi-tor). Wiley, Hoboken, NJ, Chap. 22.Volborth, A. 1979a. In Analytical Methods for Coal and Coal Products, Vol. 3, C. Karr,Jr. (Editor). Academic Press, San Diego, CA, Chap. 47.Volborth, A. 1979b. In Analytical Methods for Coal and Coal Products, Vol. 3, C. Karr,Jr. (Editor). Academic Press, San Diego, CA, Chap. 55.Volborth, A., Dahy, J. P., and Miller, G. E. 1987. In Coal Science and Chemistry,A. Volborth (Editor). Elsevier, Amsterdam, p. 417.